### Standard Test Method for Density (Unit Weight), Yield, Cement Content, and Air Content (Gravimetric) of Controlled Low-Strength Material (CLSM)

 Format Pages Price PDF 4 \$52.00 ADD TO CART

Active (view current version of standard)

Other Historical Standards

Work Item(s) - proposed revisions of this standard

1. Scope

1.1 This test method explains determination of the density (Note 1) of freshly mixed Controlled Low-Strength Material (CLSM) and gives formulas for calculating the yield, cement content, and the air content of the CLSM. This test method is based on Test Method C138/C138M for Concrete.

Note 1: Unit Weight was the previous terminology used to describe the property determined by this test method, which is mass per unit volume.

1.2 All observed and calculated values shall conform to the guidelines for significant digits and rounding established in Practice D6026.

1.2.1 The procedures used to specify how data are collected/recorded and calculated in the standard are regarded as the industry standard. In addition, they are representative of the significant digits that generally should be retained. The procedures used do not consider material variation, purpose for obtaining the data, special purpose studies, or any considerations for the user’s objectives; and it is common practice to increase or reduce significant digits of reported data to be commensurate with these considerations. It is beyond the scope of these test methods to consider significant digits used in analysis methods for engineering data.

1.3 The values stated in SI units are to be regarded as standard. The values given in parentheses are mathematical conversions to inch-pound units, which are provided for information only and are not considered standard. Reporting of test results in units other than SI shall not be regarded as nonconformance with this test method.

1.3.1 The converted inch-pound units use the gravitational system of units. In this system, the pound (lbf) represents a unit of force (weight), while the unit for mass is slugs. The converted slug is not given, unless dynamic (F=ma) calculations are involved.

1.3.2 It is common practice in the engineering/construction profession to concurrently use pounds to represent both a unit of mass (lbm) and of force (lbf). This implicitly combines two separate system of units; that is, the absolute system and the gravitational system. It is scientifically undesirable to combine the use of two separate sets of inch-pound units within a single standard. As stated, this standard includes the gravitational system of inch-pound units and does not use/present the slug unit for mass. However, the use of balances or scales recording pounds of mass (lbm) or recording density in lbm/ft3 shall not be regarded as nonconformance with this standard.

1.4 CLSM is also known as flowable fill, controlled density fill, soil-cement slurry, soil-cement grout, unshrinkable fill, “K-Krete,” and other similar names.

1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. (Warning—Fresh hydraulic cementitious mixtures are caustic and may cause chemical burns to skin and tissue upon prolonged exposure.2)

2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.

ASTM Standards

C29/C29M Test Method for Bulk Density (Unit Weight) and Voids in Aggregate

C125 Terminology Relating to Concrete and Concrete Aggregates

C128 Test Method for Relative Density (Specific Gravity) and Absorption of Fine Aggregate

C138/C138M Test Method for Density (Unit Weight), Yield, and Air Content (Gravimetric) of Concrete

C150/C150M Specification for Portland Cement

C231/C231M Test Method for Air Content of Freshly Mixed Concrete by the Pressure Method

D653 Terminology Relating to Soil, Rock, and Contained Fluids

D3740 Practice for Minimum Requirements for Agencies Engaged in Testing and/or Inspection of Soil and Rock as Used in Engineering Design and Construction

D4832 Test Method for Preparation and Testing of Controlled Low Strength Material (CLSM) Test Cylinders

D5971/D5971M Practice for Sampling Freshly Mixed Controlled Low-Strength Material

D6024/D6024M Test Method for Ball Drop on Controlled Low Strength Material (CLSM) to Determine Suitability for Load Application

D6026 Practice for Using Significant Digits in Geotechnical Data

D6103 Test Method for Flow Consistency of Controlled Low Strength Material (CLSM)

ICS Code

ICS Number Code 91.100.10 (Cement. Gypsum. Lime. Mortar)

UNSPSC Code

UNSPSC Code 30121900(Soil stabilizers and reinforcing materials)

##### Referencing This Standard
 Link Here Link to Active (This link will always route to the current Active version of the standard.)

DOI: 10.1520/D6023-15

Citation Format

ASTM D6023-15, Standard Test Method for Density (Unit Weight), Yield, Cement Content, and Air Content (Gravimetric) of Controlled Low-Strength Material (CLSM), ASTM International, West Conshohocken, PA, 2015, www.astm.org